Presentation on theme: "MICROFLEX Project - Microtechnology in Smart Fabrics Prof Steve Beeby EEE Research Group CIMTEC 2012 12 th June 2012 S Beeby, R Torah, K Yang, Y Wei, J."— Presentation transcript:
MICROFLEX Project - Microtechnology in Smart Fabrics Prof Steve Beeby EEE Research Group CIMTEC th June 2012 S Beeby, R Torah, K Yang, Y Wei, J Tudor Electronics and Computer Science
Overview Introduction to MicroFlex Functional Inks Development –Case Study 1: Printed heater on fabric –Case Study 2: Printed strain gauge on fabric –Case Study 3: Printed piezoelectrics on fabric Mechanical Microstructures on Fabric Conclusions 2
Research at Southampton 3 ECS was founded over 60 years ago 100 academic staff (36 professors) 140 research fellows, 250 PhD students Research grant income: > £12 million p.a. Over 20 years experience in developing printable active materials 3 ongoing research projects on smart fabrics (2 more completed): Microflex (EU Integrated Project) Energy Harvesting Materials for SFIT (EPSRC) Fabric based medical device (Wessex Medical) £100 million Mountbatten Building, housing state of the art cleanroom.
MicroFlex Project 4 The MicroFlex Project is a EU FP 7 funded integrated project, 7.7 M€ Budget, 5.4 M€ funding. 4 Year project, end date 30 th October Partners, 7 industrial, 9 countries. Develop MEMS processing capability for the production of flexible smart fabrics. Based on screen and inkjet printing. Develop new functional inks to be compatible with fabrics. Produce industrial prototypes demonstrating the functionality of the new inks.
55 Envisaged Process Flow Screen printing Curing Ink jet printing MEMs on fabric Fabric Functional inks Lab trials Design & simulation Active material Sacrificial layer removal process
6 Example Functions and Applications 6 Mechanical action Lighting Sensor Drug delivery Medical Transport Workwear Consumer Smart bandage, auto sterilization uniform, active monitoring underwear Luminous cabin, smart driver seat, auto clean filters Danger warning workwear (heating suite, high visibility, gas sensing, temperature sensing, movement sensing, alarm sounder Massage and cooling/heating armchair, surroundings customisation
7 Screen Printing 7 Substrate Mesh Mask Squeegee a)b) c) d) ink Also known as thick-film printing, this is normally used in the fabrication of hybridised circuits and in the manufacture of semiconductor packages.
Inkjet Printing 8 Non contact direct printing onto substrate, used for fabrics and electronics applications.
Functional Inks Development Research underpinned by novel ink development Inks need to be flexible, low temperature and robust Numerous ink types are required: 9 PassiveBasic functionalAdvanced functional Interface layerConductivePiezoresistive Encapsulation layerDielectricPiezoelectric StructuralElectroluminescent SacrificialGas sensitive Semiconducting
Case Study 1: Printed Heater Simple heater is a current carrying conductive element. Existing heaters integrated in textiles by weaving or knitting. 10 Heated Car Seat element BMW (www.bmw.com) Woven approach limited by direction of warp and weft. Knitted solution requires specialist equipment.
Interface layer Overcomes surface roughness and pilosity of fabric substrate providing a continuous planar surface for subsequent printed layers. 11 Cross-section SEM micrograph of 4 screen printed interface layers on polyester cotton fabric
Heater Design Heater printed on a fabric area of 10 x 10 cm. Heater should be flexible and maintain the properties of the fabric as much as possible. Chosen track width of 1 mm for good compromise between conduction and flexibility. Heater area coverage should be a maximum of 50% of the fabric. 12 Total track length of mm. Total area coverage for the heater = mm 2. Percentage coverage = 20.5%
Screen Design 13 Heater has three layers: Interface, Conductor and Encapsulation. Interface layer improves heater performance but increases fabric coverage to ~40% - still below limit of 50%. Fabric Interface layer Conductor layer Encapsulation layer 10cm Interface screen Conductor screen Complete design
Influence of Interface Layer 15 Printed track calculated sheet resistance for each substrate Interface Fabric Alumina Printed track on each substrate 80 mΩ/sq 194 mΩ/sq 50 mΩ/sq
Results o C heating achieved with 30 V and current limit of 200 mA. Increases to 120 o C after 15 minutes with 600 mA current limit. Fabric temperature within 2% of track temperature. Low pattern percentage ensures fabric remains flexible and maintains key fabric properties such as breathability and wearer comfort.
Case Study 2: Strain Gauge Printed strain gauge demonstrated by project partners Jožef Stefan Institute, ink developed by ITCF and fabric from Saati. Exploits the piezoresistive effect: the resistance of a printed film changes as it is strained (stretched) due to a change in the resistivity of the material. Useful for sensing movement, forces and strains. 17
Printed Sensor 18 Silver electrodes printed using a low temperature polymer silver paste. Piezoresistive paste is based on graphite. Cured at o C 1 print2 prints 3 prints
Results Sensitivity illustrated by the Gauge factor: Clear increase in resistance demonstrated as the fabric is strained. Conventional metal foil GF = 2 19 N° of graphite layer R 0 (Ω) at 0 % strain R(Ω) at 1.5 % strain Gauge factor
Strain vs Load By measuring resistance the load on the fabric can be calculated. 20 B. Perc, et al. ‘Thick-film strain sensor on textiles’, 45th International Conference on Microelectronics, Devices and Materials - MIDEM, Slovenia 9-11 Sept 2009.
21 Case Study 3: Piezoelectric Films Piezoelectric materials expand when subject to an electrical field, similarly they produce an electrical charge when strained. Ideal material for sensing and actuating applications. Meggitt have developed a screen printable piezoelectric paste that can be printed onto fabrics.
22 Piezoelectric Structure Piezoelectric material sandwiched between electrodes. Polarising voltage required after printing to make the piezoelectric active. Cured at temperatures below 150 o C. Promising sensitivity demonstrated (d 33 ~ 30 pC/N) 22 Images courtesy of Meggitt Sensing Systems
23 Printed MEMS The MicroFlex project is concentrating on fabricating sensors and actuators (transducers) and developing printed MEMS. MicroFlex aims to use standard printing techniques and custom inks in order to realise freestanding mechanical structures coupled with active films for sensing and actuating. Developed a surface micromachining process for printed films on fabrics
Printed MEMS Process 24 Piezoresistive layer Interface layer Sacrificial layer Structural layer Fabric Electrode Sacrificial layer requirements: printable, solid, compatible, can be easily removed without damaging fabric or other layers. Structural layer requirements: suitable mechanical/functional properties.
Process Requirements Implemented by screen printing. Sacrificial technology: removal method must be compatible with fabrics i.e. low temperature, non solvent based. Structural material and its processing must be compatible with the sacrificial material. Structural materials properties chosen for the particular application. 25
Sacrificial Material and Process Plastic crystal (Trimethylolethane, TME): –An intermediate solid form between the real solid and liquid forms –Sublimation instead of liquefaction Sublimation starts around 87 o C Low curing and removal temperatures –Curing: o C –Removal: o C 27
Results Sacrificial layer was completely removed at 160 o C. No visible damage to fabric properties 28 Resonance test shows cantilever was fully undercut, and results match FEA.
Piezoelectric Cantilever Piezoelectric version also fabricated 29 Film thicknesses: Interface layer ~100 m Sacrificial layer ~100 m Structural layer ~80 m Electrodes ~15 m PZT m Voltage versus frequency for different acceleration levels.
Micropump Initially printed on Kapton, demonstrates sacrificial process combined with structural, conductive and piezoelectric films. Uses passive nozzle/diffuser valves, achieves 27 uL/min from 100 V P-P at 1 MHz, pumping IPA. 30 Chamber Top electrode Bottom electrode PZT layer Flow path
Conclusions MicroFlex has developed the materials and processes required to fabricate printed MEMS on fabrics. Wide range of active inks have been developed. Numerous prototypes based upon these active inks demonstrated. Sacrificial layer fabrication process has also been demonstrated and is being applied to several structures and devices including accelerometers, pressure sensors and micropumps. 31
Smart Fabric Inks Ltd Company launched February 2011 Marketing inks developed at the University of Southampton Please visit for further informationwww.fabinks.com 32
Acknowledgements 33 Colleagues at Southampton, MicroFlex partners and EU for funding (CP-IP ). Thanks for your attention!